Presentation on theme: "MECHANICAL PROPERTIES OF MATERIALS Manufacturing Processes, 1311 Dr Simin Nasseri Southern Polytechnic State University."— Presentation transcript:
MECHANICAL PROPERTIES OF MATERIALS Manufacturing Processes, 1311 Dr Simin Nasseri Southern Polytechnic State University
Manufacturing Processes Prof Simin Nasseri MECHANICAL PROPERTIES OF MATERIALS 1.Bending Test (Slide 3)Slide 3 2.Shear Test (Slide 8)Slide 8 3.Hardness (Slide 14)Slide 14 4.Effect of Temperature on Properties (Slide 20)Slide 20 5.Fluid Properties (Slide 26)Slide 26 6.Viscoelastic Behavior of Polymers (Slide 34)Slide 34
Manufacturing Processes Prof Simin Nasseri Bending Test (also called flexure test) Specimen of rectangular cross section is positioned between two supports, and a load is applied at its center Figure 3.10 Bending of a rectangular cross section results in both tensile and compressive stresses in the material: (1) initial loading; (2) highly stressed and strained specimen; and (3) bent part.
Manufacturing Processes Prof Simin Nasseri Bending Test 3-point and 4-point bending tests:
Manufacturing Processes Prof Simin Nasseri Testing of Brittle Materials Hard brittle materials (e.g., ceramics) possess elasticity but little or no plasticity Often tested by a bending test Brittle materials do not flex They deform elastically until fracture Failure occurs because tensile strength of outer fibers of specimen are exceeded Failure type: cleavage - common with ceramics and metals at low temperatures, in which separation rather than slip occurs along certain crystallographic planes
Manufacturing Processes Prof Simin Nasseri Transverse Rupture Strength The strength value derived from the bending test: where TRS = Transverse Rupture Strength; F = applied load at fracture; L = length of specimen between supports; and b and t are dimensions of cross-section
Manufacturing Processes Prof Simin Nasseri Shear Test (also known as torsion test) Application of stresses in opposite directions on either side of a thin element Figure 3.11 Shear (a) stress and (b) strain.
Manufacturing Processes Prof Simin Nasseri Shear Test Deform a matchbox and see the deformations in all sides of the box. The area over which the deflection occurs is the area of consideration. A F F A
Manufacturing Processes Prof Simin Nasseri Shear Stress and Strain Shear stress defined as where F = applied force; and A = area over which deflection occurs. Shear strain defined as where = deflection element; and b = distance over which deflection occurs
Manufacturing Processes Prof Simin Nasseri Torsion Stress-Strain Curve Figure 3.13 Typical shear stress strain curve from a torsion test.
Manufacturing Processes Prof Simin Nasseri Shear Elastic Stress Strain Relationship In the elastic region, the relationship is defined as where G = shear modulus, or shear modulus of elasticity For most materials, G 0.4E, where E = elastic modulus
Manufacturing Processes Prof Simin Nasseri Shear Plastic Stress Strain Relationship Relationship similar to flow curve for a tensile test Shear stress at fracture = shear strength S Shear strength can be estimated from tensile strength: S 0.7(TS) Since cross sectional area of test specimen in torsion test does not change as in tensile and compression, engineering stress strain curve for shear true stress strain curve
Manufacturing Processes Prof Simin Nasseri Hardness Resistance to permanent indentation Good hardness generally means material is resistant to scratching and wear Most tooling used in manufacturing must be hard for scratch and wear resistance
Manufacturing Processes Prof Simin Nasseri Hardness Tests Commonly used for assessing material properties because they are quick and convenient Variety of testing methods are appropriate due to differences in hardness among different materials Most well known hardness tests are Brinell and Rockwell Other test methods are also available, such as Vickers, Knoop, Scleroscope, and durometer
Manufacturing Processes Prof Simin Nasseri Widely used for testing metals and nonmetals of low to medium hardness A hard ball is pressed into specimen surface with a load of 500, 1500, or 3000 kg Figure 3.14 Hardness testing methods: (a) Brinell Brinell Hardness Test
Manufacturing Processes Prof Simin Nasseri Brinell Hardness Number Load divided into indentation area = Brinell Hardness Number (BHN) where HB = Brinell Hardness Number (BHN), F = indentation load, kg; D b = diameter of ball, mm, and D i = diameter of indentation, mm
Manufacturing Processes Prof Simin Nasseri Brinell Hardness Number Lets work on two extreme cases: D i is extremely low (lets consider it as zero!): This means that if there is almost no indentation, the material is extremely hard! In case D i = D b (the whole ball is inserted into the specimen): A * is the area of the semisphere. This means that HB number is in fact the force divided by the area of contact!
Manufacturing Processes Prof Simin Nasseri Rockwell Hardness Test Another widely used test A cone shaped indenter is pressed into specimen using a minor load of 10 kg, thus seating indenter in material Then, a major load of 150 kg is applied, causing indenter to penetrate beyond its initial position Additional penetration distance d is converted into a Rockwell hardness reading by the testing machine Figure 3.14 Hardness testing methods: (b) Rockwell: (1) initial minor load and (2) major load.
Effect of Temperature on Properties
Manufacturing Processes Prof Simin Nasseri Effect of Temperature on Properties Figure 3.15 General effect of temperature on strength and ductility.
Manufacturing Processes Prof Simin Nasseri Hot Hardness Ability of a material to retain hardness at elevated temperatures Figure 3.16 Hot hardness typical hardness as a function of temperature for several materials.
Manufacturing Processes Prof Simin Nasseri Recrystallization in Metals Most metals strain-harden at room temperature according to the flow curve (n > 0) But if heated to sufficiently high temperature and deformed, strain hardening does not occur Instead, new grains are formed that are free of strain The metal behaves as a perfectly plastic material; that is, n = 0
Manufacturing Processes Prof Simin Nasseri Recrystallization Temperature Formation of new strain free grains is called recrystallization Recrystallization temperature of a given metal = about one half its melting point (0.5 T m ) as measured on an absolute temperature scale Recrystallization takes time - the recrystallization temperature is specified as the temperature at which new grains are formed in about one hour
Manufacturing Processes Prof Simin Nasseri Recrystallization and Manufacturing Heating a metal to its recrystallization temperature prior to deformation allows a greater amount of straining, and lower forces and power are required to perform the process Forming metals at temperatures above recrystallization temperature is called hot working
Fluid Properties and Manufacturing
Manufacturing Processes Prof Simin Nasseri Fluid Properties and Manufacturing Fluids flow - They take the shape of the container that holds them Many manufacturing processes are accomplished on materials converted from solid to liquid by heating Called solidification processes Examples: Metals are cast in molten state Glass is formed in a heated and fluid state Polymers are almost always shaped as fluids
Manufacturing Processes Prof Simin Nasseri Viscosity in Fluids Viscosity is the resistance to flow that is characteristic of a given fluid Flow is a defining characteristic of fluids, but the tendency to flow varies for different fluids Viscosity is a measure of the internal friction when velocity gradients are present in the fluid The more viscous the fluid, the higher the internal friction and the greater the resistance to flow Reciprocal of viscosity is fluidity the ease with which a fluid flows
Manufacturing Processes Prof Simin Nasseri Viscosity Viscosity can be defined using two parallel plates separated by a distance d and a fluid fills the space between the two plates Figure 3.17 Fluid flow between two parallel plates, one stationary and the other moving at velocity v
Manufacturing Processes Prof Simin Nasseri Shear Stress Shear stress is the frictional force exerted by the fluid per unit area Motion of the upper plate is resisted by a frictional force resulting from the shear viscosity of the fluid This force F can be reduced to a shear stress by dividing by plate area A
Manufacturing Processes Prof Simin Nasseri Shear Rate Shear stress is related to shear rate, defined as the change in velocity dv relative to dy where = shear rate, [1/s]; dv = change in velocity, [m/s]; and dy = change in distance y, [m] Shear rate = velocity gradient perpendicular to flow direction
Manufacturing Processes Prof Simin Nasseri Shear Viscosity Shear viscosity is the fluid property that defines the relationship between F/A and dv/dy; that is, or where = a constant of proportionality called the coefficient of viscosity, [Pa-s] For Newtonian fluids, viscosity is a constant For non-Newtonian fluids, it is not
Manufacturing Processes Prof Simin Nasseri Coefficient of Viscosity Rearranging, Shear viscosity (also called coefficient of viscosity) can be expressed: Viscosity of a fluid is the ratio of shear stress to shear rate during flow
Viscosity of Polymers and Flow Rate
Manufacturing Processes Prof Simin Nasseri Viscosity of Polymers and Flow Rate Viscosity of a thermoplastic polymer melt is not constant It is affected by flow rate Its behavior is non-Newtonian A fluid that exhibits this decreasing viscosity with increasing shear rate is called pseudoplastic This complicates analysis of polymer shaping processes such as injection molding
Manufacturing Processes Prof Simin Nasseri Newtonian versus Pseudoplastic Fluids Figure 3.18 Viscous behaviors of Newtonian and pseudoplastic fluids. Polymer melts exhibit pseudoplastic behavior. For comparison, the behavior of a plastic solid material is shown.
Manufacturing Processes Prof Simin Nasseri Viscoelastic Behavior Material property that determines the strain that the material experiences when subjected to combinations of stress and temperature over time Combination of viscosity and elasticity
Manufacturing Processes Prof Simin Nasseri Elastic versus Viscoelastic Behavior Figure 3.19 (a) perfectly elastic response of material to stress applied over time; and (b) response of a viscoelastic material under same conditions. The material in (b) takes a strain that is a function of time and temperature.
Manufacturing Processes Prof Simin Nasseri Viscoelastic Behavior of Polymers: Shape Memory A problem in extrusion of polymers is die swell, in which the profile of extruded material grows in size, reflecting its tendency to return to its previously larger cross section in the extruder barrel immediately before being squeezed through the smaller die opening